J Adv Prosthodont 2017;9:118-23
The effect of plasma on shear bond strength between resin cement and colored zirconia Chan Park†, Seung-Hwan Yoo†, Sang-Won Park, Kwi-Dug Yun, Min-Kyung Ji, Jin-Ho Shin, Hyun-Pil Lim* Department of Prosthodontics, School of Dentistry, Chonnam National University, Gwangju, Republic of Korea
PURPOSE. To investigate the effect of non-thermal atmospheric pressure plasma (NTAPP) treatment on shear bond strength (SBS) between resin cement and colored zirconia made with metal chlorides. MATERIALS AND METHODS. 60 zirconia specimens were divided into 3 groups using coloring liquid. Each group was divided again into 2 sub-groups using plasma treatment; the experimental group was treated with plasma, and the control group was untreated. The sub-groups were: N (non-colored), C (0.1 wt% aqueous chromium chloride solution), M (0.1 wt% aqueous molybdenum chloride solution), NP (non-colored with plasma), CP (0.1 wt% aqueous chromium chloride solution with plasma), and MP (0.1 wt% aqueous molybdenum chloride solution with plasma). Composite resin cylinders were bonded to zirconia specimens with MDP-based resin cement, and SBS was measured using a universal testing machine. All data was analyzed statistically using a 2-way ANOVA test and a Tukey test. RESULTS. SBS significantly increased when specimens were treated with NTAPP regardless of coloring (P .05) (Table 3). The mean (± SD) MPa values for N group, C group, and M group were 4.24 ± 0.334, 3.79 ± 0.367, and 5.12 ± 0.181, respectively. One-way ANOVA confirmed that the SBS for each group differed significantly (P < .001). The post-hoc Tukey HSD test confirmed a significant difference between chromium group (P < .05) and molybdenum group (P < .001) compared with non-colored group (Fig. 3). The SBS values for NP group, CP group, and MP group were 6.46 ± 0.372, 5.89 ± 0.237, and 7.29 ± 1.082 MPa, respectively, and additional statistical analysis indicated significant differences among the specimens (P < .001). Results of Tukey’s HSD test showed no significant difference between non-colored with plasma group and chromium with plasma group, whereas molybdenum with plasma group exhibited a significantly higher SBS (Fig. 4). Independent t-tests, to compare SBS values with respect to NTAPP in each group, confirmed a significant increase in the average SBS for all groups (P < .001) (Fig. 5). Fig. 6 shows representative SEM images of fractured surface. All groups showed adhesive failure mode.
Table 3. Two-way ANOVA test results of effects between subjects Source
Sum of squares
Type of specimen
NTAPP x Type of specimen
(*: Significant at P < .05)
The effect of plasma on shear bond strength between resin cement and colored zirconia
Fig. 3. Result of Tukey HSD test for shear bond strength before plasma treatment (* : significant at P < .05, **: significant at P < .001).
Fig. 4. Result of Tukey HSD test for shear bond strength after plasma treatment (* : significant at P < .05).
Fig. 5. Result of Independent t-test for shear bond strength (** : significant at P < .001).
Fig. 6. SEM representative image of specimen fractured surfaces (×180 magnification). (A) Non-colored, (B) Noncolored with plasma, (C) Chromium colored, (D) Chromium colored with plasma, (E) Molybdenum colored, (F) Molybdenum colored with plasma (R is composite resin, Z is zirconia specimen). The Journal of Advanced Prosthodontics
J Adv Prosthodont 2017;9:118-23
Discussion The aim of this study was to evaluate the effect of NTAPP treatment on SBS between colored zirconia and a type of MDP-based resin cement. The results showed that SBS increased significantly among the specimens treated with NTAPP. Thus, the first null hypothesis could be rejected. Moreover, the NTAPP-treated zirconia specimens showed statistically significant difference in SBS, independent of whether they had been colored or not. However, SBS on NTAPP-treated colored zirconia was higher than non-colored zirconia, and so the second null hypothesis was rejected. Cales16 reported that specific coloring of zirconia could be achieved by adding different metal oxides. On the other hand, Oh et al.5 used metal chloride to color zirconia by means of the liquid immersion method. When adding metal chloride to color the zirconia, an oxygen vacancy is produced, replacing zirconium with a transition metal ion. Oxide is formed when the disassembled oxygen atom combines with the transition metal.4,17 Oh et al.5 produced chloride-colored zirconia that showed improved mechanical properties and biocompatibility. From among the various metal chlorides, we chose 0.1 wt% aqueous chromium chloride solution and 0.1 wt% aqueous molybdenum chloride solution, because they can both simulate natural tooth shades but do not cause cytotoxicity.4,5 In a previous study,6 zirconia specimens that were immersed in aqueous molybdenum chloride solution showed significantly higher SBS values, compared with other specimens, as aqueous molybdenum chloride solution changed the granular boundary of zirconia unevenly. This phenomenon that changed zirconia particle size and morphology enhanced the abrasion resistance, tensile strength, stability, and bond strength.18-20 Dental cement plays an important role in restoration longevity by improving the retention of the restoration. A previous study18 reported that the bond strength of zirconia depended upon the type of cement used, regardless of the surface treatment. Many researchers have found that the use of Panavia F 2.0 with MDP-based resin cement can increase SBS with zirconia;19-21 and for this reason, we used Panavia F 2.0 in our study. As zirconia lacks a silica component, it is generally not subjected to acid etching, which is performed prior to resin bonding. In contrast to feldspathic porcelain, zirconia bonding is more difficult, and many methods have been attempted to improve it. However, our study was not an attempt to increase mechanical bonding to determine the distinct effects of plasma treatment. Plasma treatment produces a chemically altered surface on certain materials to facilitate the formation of peroxide radicals (R-O-O).24-27 The functional groups on the altered zirconia surface can combine with phosphate (C=O) in the resin cement, thus increasing the bond strength between the cement and the zirconia. 28 Also, the plasma treatment enhances chemical bonding by introducing a secondary force, according to the Van der Waals equation.29 In addition, in the case of plasma, a previous study30 indicated that 122
the decrease in bonding strength, as a result of polluted organic material in zirconia, can be overcome by increasing the plasma’s cleansing potential by decreasing the absorbed hydrocarbon through severing the bond between C-H and C-C. Although SBS was higher with NTAPP treatment than without it, our subsequent analysis of the failure modes under FE-SEM (S-4700, Hitachi Ltd., Tokyo, Japan) showed that all specimens were presented adhesive failure mode. Our results here suggest that this phenomenon warrants additional study. Many studies in which zirconia is being treated with NTAPP are underway, however the specific application of NTAPP to colored zirconia using metal chloride still requires investigation. We confirmed that the physical and chemical features of colored zirconia remain stable with such treatment, since there was no significant difference in the response of non-colored zirconia when compared to the colored zirconia. In particular, colored zirconia immersed in 0.1 wt% aqueous molybdenum chloride solution can potentially be utilized in many fields, because SBS is greatly increased by the application of NTAPP. Meanwhile, the NTAPP-treated colored zirconia immersed in 0.1 wt% aqueous molybdenum chloride solution showed the highest standard deviation, which means the mechanism of this phenomenon remains to be determined. Additionally, for the best potential clinical applications, future experiments to assess the type of gas used for the plasma treatment, optimum processing times, and combinations with other surface treatments, should be undertaken.
Conclusion Within the limitations of this study, SBS between zirconia and resin cement was improved when NTAPP treatment was applied to colored zirconia. In particular, colored zirconia with molybdenum showed a higher SBS compared to other zirconia types before and after processing with NTAPP.
ORCID Chan Park http://orcid.org/0000-0001-5729-5127 Seung-Hwan Yoo http://orcid.org/0000-0002-5640-9468 Sang-Won Park http://orcid.org/0000-0002-9376-9104 Kwi-Dug Yun http://orcid.org/0000-0002-2965-3967 Min-Kyung Ji http://orcid.org/0000-0002-3525-644X Jin-Ho Shin http://orcid.org/0000-0003-2072-0614 Hyun-Pil Lim http://orcid.org/0000-0001-5586-1404
References 1. Preis V, Behr M, Kolbeck C, Hahnel S, Handel G, Rosentritt M. Wear performance of substructure ceramics and veneering porcelains. Dent Mater 2011;27:796-804. 2. Aboushelib MN, de Jager N, Kleverlaan CJ, Feilzer AJ. Microtensile bond strength of different components of core
The effect of plasma on shear bond strength between resin cement and colored zirconia
veneered all-ceramic restorations. Dent Mater 2005;21:984-91. 3. Heffernan MJ, Aquilino SA, Diaz-Arnold AM, Haselton DR, Stanford CM, Vargas MA. Relative translucency of six all-ceramic systems. Part II: core and veneer materials. J Prosthet Dent 2002;88:10-5. 4. Yuan JC, Brewer JD, Monaco EA Jr, Davis EL. Defining a natural tooth color space based on a 3-dimensional shade system. J Prosthet Dent 2007;98:110-9. 5. Oh GJ, Lee KM, Lee DJ, Lim HP, Yun KD, Ban JS, Lee KK, Fisher JG, Park SW. Effect of metal chloride solutions on coloration and biaxial flexural strength of yttria-stabilized zirconia. Met Mater Int 2012;18:805-12. 6. Kim GH, Park SW, Lee K, Oh GJ, Lim HP. Shear bond strength between resin cement and colored zirconia made with metal chlorides. J Prosthet Dent 2015;113:603-8. 7. Behr M, Proff P, Kolbeck C, Langrieger S, Kunze J, Handel G, Rosentritt M. The bond strength of the resin-to-zirconia interface using different bonding concepts. J Mech Behav Biomed Mater 2011;4:2-8. 8. Chang JC, Powers JM, Hart D. Bond strength of composite to alloy treated with bonding systems. J Prosthodont 1993;2: 110-4. 9. Blatz MB, Sadan A, Martin J, Lang B. In vitro evaluation of shear bond strengths of resin to densely-sintered high-purity zirconium-oxide ceramic after long-term storage and thermal cycling. J Prosthet Dent 2004;91:356-62. 10. Phark JH, Duarte S Jr, Blatz M, Sadan A. An in vitro evaluation of the long-term resin bond to a new densely sintered high-purity zirconium-oxide ceramic surface. J Prosthet Dent 2009;101:29-38. 11. von Woedtke T, Metelmann HR, Weltmann KD. Clinical plasma medicine: state and perspectives of in vivo application of cold atmospheric plasma. Contributions Plasma Phys 2014; 54:104-17. 12. Derand T, Molin M, Kvam K. Bond strength of composite luting cement to zirconia ceramic surfaces. Dent Mater 2005; 21:1158-62. 13. Canullo L, Micarelli C, Bettazzoni L, Koçi B, Baldissara P. Zirconia-composite bonding after plasma of argon treatment. Int J Prosthodont 2014;27:267-9. 14. Shim JW, Lee K, Jeong MJ, Jung SC, Kim BH. Hyaluronic acid immobilization on the poly-allylamine coated nano-network TiO2 surface. J Nanosci Nanotechnol 2011;11:7343-6. 15. Rammelt S, Illert T, Bierbaum S, Scharnweber D, Zwipp H, Schneiders W. Coating of titanium implants with collagen, RGD peptide and chondroitin sulfate. Biomaterials 2006;27: 5561-71. 16. Cales B. Colored zirconia ceramics for dental applications. Bioceram 1998;11:591-4. 17. Shah K, Holloway JA, Denry IL. Effect of coloring with various metal oxides on the microstructure, color, and flexural strength of 3Y-TZP. J Biomed Mater Res B Appl Biomater 2008;87:329-37. 18. Ueno T, Kumagai T, Hirota K,Saitoh Y, Kojima I. The characteristic of metal adhesion primer GC Metal Primer II. J Dent Res 1997;76:312. 19. Beuer F, Erdelt K, Schweiger J, Eichberger M. Flexural
strength of coloured and aged zirconia. J Dent Res 2004;83: 942-54. 20. Bartolomé JF, Díaz M, Moya JS. Influence of the metal particle size on the crack growth resistance in mullite-molybdenum composites. J Am Ceram Soc 2002;85:2778-84. 21. Sbaizero O, Roitti S, Pezzotti G. R-curve behavior of alumina toughened with molybdenum and zirconia particles. Mat Sci Eng A 2003;359:297-302. 22. Khan AA, Labbe JC. Aluminium nitride–molybdenum ceramic matrix composites: influence of molybdenum concentration on the mechanical properties. J Mater Sci 1997;32:382933. 23. Ozcan M, Vallittu PK. Effect of surface conditioning methods on the bond strength of luting cement to ceramics. Dent Mater 2003;19:725-31. 24. Kern M, Wegner SM. Bonding to zirconia ceramic: adhesion methods and their durability. Dent Mater 1998;14:64-71. 25. Wegner SM, Gerdes W, Kern M. Effect of different artificial aging conditions on ceramic-composite bond strength. Int J Prosthodont 2002;15:267-72. 26. Lüthy H, Loeffel O, Hammerle CH. Effect of thermocycling on bond strength of luting cements to zirconia ceramic. Dent Mater 2006;22:195-200. 27. Silva NR, Coelho PG, Valverde GB, Becker K, Ihrke R, Quade A, Thompson VP. Surface characterization of Ti and Y-TZP following non-thermal plasma exposure. J Biomed Mater Res B Appl Biomater 2011;99:199-206. 28. Kim JH, Lee MA, Han GJ, Cho BH. Plasma in dentistry: a review of basic concepts and applications in dentistry. Acta Odontol Scand 2014;72:1-12. 29. Zhang W, Chu PK, Ji J, Zhang Y, Liu X, Fu RK, Ha PC, Yan Q. Plasma surface modification of poly vinyl chloride for improvement of antibacterial properties. Biomaterials 2006;27: 44-51. 30. Yavirach P, Chaijareenont P, Boonyawan D, Pattamapun K, Tunma S, Takahashi H, Arksornnukit M. Effects of plasma treatment on the shear bond strength between fiber-reinforced composite posts and resin composite for core buildup. Dent Mater J 2009;28:686-92. 31. Yoshida K, Tsuo Y, Atsuta M. Bonding of dual-cured resin cement to zirconia ceramic using phosphate acid ester monomer and zirconate coupler. J Biomed Mater Res B Appl Biomater 2006;77:28-33. 32. Valverde GB, Coelho PG, Janal MN, Lorenzoni FC, Carvalho RM, Thompson VP, Weltemann KD, Silva NR. Surface characterisation and bonding of Y-TZP following non-thermal plasma treatment. J Dent 2013;41:51-9. 33. Amaral R, Ozcan M, Bottino MA, Valandro LF. Microtensile bond strength of a resin cement to glass infiltrated zirconiareinforced ceramic: the effect of surface conditioning. Dent Mater 2006;22:283-90.
The Journal of Advanced Prosthodontics